A single-crystal to single-crystal phase transition in [Co(NH3)5NO2]Br2at high pressure: a step towards understanding linkage photo-isomerisation
Zakharov, B. A.; Marchuk, A. S.; Boldyreva, E. V.; CrystEngComm 17 (2015) 8812–; doi:10.1039/C5CE01820J

data_7223046
_publ_section_title
;
 A single-crystal to single-crystal phase transition in [Co(NH3)5NO2]Br2at
 high pressure: a step towards understanding linkage photo-isomerisation
;
_journal_issue                   46
_journal_name_full               CrystEngComm
_journal_page_first              8812
_journal_paper_doi               10.1039/C5CE01820J
_journal_volume                  17
_journal_year                    2015
_chemical_formula_moiety         'Co H15 N6 O2, 2(Br)'
_chemical_formula_sum            'Br2 Co H15 N6 O2'
_chemical_formula_weight         349.93
_chemical_name_common            nitro-pentaammine-Co(III)-dibromide
_chemical_name_systematic        nitro-pentaammine-Co(III)-dibromide
_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_Hall           '-C 2yc'
_space_group_name_H-M_alt        'C 1 2/c 1'
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2015-09-10 deposited with the CCDC.
2015-10-25 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 93.439(4)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   10.6023(5)
_cell_length_b                   7.5308(7)
_cell_length_c                   10.6049(4)
_cell_measurement_reflns_used    1704
_cell_measurement_temperature    295(2)
_cell_measurement_theta_max      27.8020
_cell_measurement_theta_min      2.6420
_cell_volume                     845.21(9)
_computing_cell_refinement
;
CrysAlisPro, Agilent Technologies,
Version 1.171.35.21 (release 20-01-2012 CrysAlis171 .NET)
(compiled Jan 23 2012,18:06:46)
;
_computing_data_collection
;
CrysAlisPro, Agilent Technologies,
Version 1.171.35.21 (release 20-01-2012 CrysAlis171 .NET)
(compiled Jan 23 2012,18:06:46)
;
_computing_data_reduction
;
CrysAlisPro, Agilent Technologies,
Version 1.171.35.21 (release 20-01-2012 CrysAlis171 .NET)
(compiled Jan 23 2012,18:06:46)
;
_computing_molecular_graphics    'Mercury (Macrae et al., 2006)'
_computing_publication_material  'enCIFer (Allen et al., 2004)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_pressure         4800000
_diffrn_ambient_temperature      295(2)
_diffrn_detector_area_resol_mean 10.3457
_diffrn_measured_fraction_theta_full 0.576
_diffrn_measured_fraction_theta_max 0.560
_diffrn_measurement_device_type  'Xcalibur, Ruby, Gemini'
_diffrn_measurement_method       \w-scan
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0546
_diffrn_reflns_av_unetI/netI     0.0335
_diffrn_reflns_laue_measured_fraction_full 0.576
_diffrn_reflns_laue_measured_fraction_max 0.560
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_l_max       13
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            2236
_diffrn_reflns_point_group_measured_fraction_full 0.576
_diffrn_reflns_point_group_measured_fraction_max 0.560
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         26.354
_diffrn_reflns_theta_min         3.320
_diffrn_source                   'Enhance (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    11.454
_exptl_absorpt_correction_T_max  0.272
_exptl_absorpt_correction_T_min  0.207
_exptl_absorpt_correction_type   gaussian
_exptl_absorpt_process_details   'Absorb-7 (Angel, 2013)'
_exptl_crystal_colour            orange
_exptl_crystal_density_diffrn    2.750
_exptl_crystal_description       block
_exptl_crystal_F_000             680
_exptl_crystal_preparation       'mounted in DAC'
_exptl_crystal_size_max          0.20
_exptl_crystal_size_mid          0.20
_exptl_crystal_size_min          0.05
_refine_diff_density_max         0.386
_refine_diff_density_min         -0.376
_refine_diff_density_rms         0.098
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.070
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     52
_refine_ls_number_reflns         482
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.070
_refine_ls_R_factor_all          0.0273
_refine_ls_R_factor_gt           0.0252
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0275P)^2^+2.5892P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0586
_refine_ls_wR_factor_ref         0.0603
_reflns_Friedel_coverage         0.000
_reflns_number_gt                451
_reflns_number_total             482
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c5ce01820j3.cif
_cod_data_source_block           480GPa
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_absorpt_correction_type' value 'Gaussian' changed to
'gaussian' according to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 3271 2015-04-21 07:52:19Z andrius 

 Adding full bibliography for 7223037--7223049.cif.
;
_cod_database_code               7223046
_shelx_shelxl_version_number     2014/7
_shelx_res_checksum              20634